EN 10216-2 Seamless steel tubes for pressure purposes – Technical delivery conditions – part 2: Non- alloy and alloy steel tubes with specified elevated temperature
This Part of EN10216 specifies the technical delivery conditions in two categories for seamless tubes of circular cross section, with specified elevated temperature properties, made of non-alloy and alloy steel.
Steel Grade: 16Mo3 Steel Number: 1.5415
Chemical composition (cast analysis)a, in % by mass
C: 0.12-0.20 b
P max: 0.025
S max: 0.020
Al total: ≤0.040
Cu: ≤0.30 c
a Elements not included in this Table shall not be intentionally added to the steel without the agreement of the purchaser, except for elements which may be added for finishing the cast. All appropriate measures shall be taken to prevent the addition of undesirable elements from scrap or other materials used in the steel making process.
b For wall thickness≥30mm the carbon content may be increased by 0.02% for cast and product analysis.
c Option: In order to facilitate subsequent forming operations, an agreed maximum copper content lower than indicated and an agreed specified maximum tin content shall apply.
Normalizing includes normalizing forming
Temperature: 890 – 950 ℃
Cooling medium: air
Tensile properties at room and below room temperature
Upper yield strength or proof strength ReH or RP0.2 for Wall Thickness T min.
Wall thickness mm
Tensile Strength, Rm, Mpa: 450 to 600
Elongation A, min. %:
Minimum average absorbed energy KV J at a temperature of 20℃
Minimum proof strength Rp0.2 Mpa at elevated temperature ℃（option）
Wall thickness, mm: ≤60
Tolerance on outside diameter and wall thickness
For outside diameter: ±1% or 0.5mm whichever is the greater
For wall thickness:
Outside Diameter D
|Tolerances on T for a T/D ratio|
12.5% or 0.4mm whichever is the greater
For outside diameter D≥355.6 mm it is permitted to exceed the upper wall thickness locally by a further 5% of the wall thickness T
Tolerance on exact lengths
|Tolerance on exact length|
|L ≤ 6000|
0, by agreement